2K Ceramic Chassis Black is our most durable, chemical-resistant, and easiest-to-spray Chassis Black yet!
- Highly chip- and abrasion-resistant
- Incredibly UV-resistant
- Dries fast
Eastwood's 2K Ceramic Chassis Black is a super-durable coating that's not only beautiful, but also tough as nails. Our proprietary formula imbeds finely ensures a high-quality 2K (2-component) 4:1 urethane base to create the ultimate, factory-correct finish. You'll need 2 quarts of Chassis Black for a full-frame vehicle.
About Eastwood 2K Ceramic Chassis Black Gloss
You asked for a tough, super-durable chassis coating, so our R&D team developed Eastwood's 2K Ceramic Chassis Black. It's a chip- and chemical-resistant coating with incredible abrasion- and UV-resistance, fast dry times and a finish that's second to none. When laid over Eastwood's 50242ZP 2K Epoxy Primer, it gives you a no-worry finish that will last and last. Withstands up to 300 degreesF. Each quart covers 50 sq. ft. in 2 coats (a full-frame vehicle requires 2 quarts).
Easy 4:1 mix with the activator included; spray with a 1.3mm or larger nozzle HVLP spray gun. For professional use only. Contains isocynates; proper respiratory protection must be used. Product information sheet - Click Here
50544ZP is the Gloss 2K Ceramic Chassis Black (1-qt.)
21854Z Activator (8-oz.) Kit
Use on full and partial frames, floor pans/undercarriages, suspension components, off-road and race vehicles, roll cages. Eastwood 2K Ceramic Chassis Black is easily applied with your HVLP spray gun using a 1.3mm or larger nozzle. Provides complete hiding in 2 coats; allow 10 minutes between coats. Refer to product label for more complete application directions and safety information. Can be applied directly over our 50242ZP Epoxy Primer (sold separately) after 60 minutes to 5 days without scuffing.
(Q) Can Eastwood 2K Ceramic Chassis Black be applied directly over other finishes?
(A) Generally 2K Ceramic Chassis Black can be applied over most thoroughly cured finishes (finishes that cannot be indented with a thumbnail). Scuff first with 320-600-grit sandpaper and test a small area before coating the entire area. If lifting occurs, remove the lifting paint, sand the surrounding area, and seal the surface by priming first with 50242ZP Epoxy Primer mixed with 50243ZP Epoxy Primer Catalyst. NOTE: Eastwood Epoxy Primer can be reduced up to 20% with 50104ZP Universal Zero-VOC Urethane Reducer to use strictly as a sealer.
Always wear appropriate eye, skin and respiratory protection when using this product. Always apply in a well ventilated area, away from open flames Consult MSDS for specific safety warnings and hazards.
Product information sheet - Click Here
Eastwood Offers Free Lifetime Technical Support
Attention California Residents - Proposition 65
WARNING - Cancer and Reproductive Harm - www.P65Warnings.ca.gov